Design and Development of Fire Resistant Steels Cameron Gross, Dieter Isheim, Semyon Vaynman, Morris E. Fine, Yip-Wah Chung ! SRG 2014 Northwestern University March 25, 2014 Enhanced structural steels • Steels need to maintain strength in building fires.! • Delay building collapse.! • Extend time of structural safety to allow for evacuation. Photo Credit: Eric Hensley, Wikimedia Commons 2 Construction standards • Current building codes: 50% of room temperature yield strength at 550°C.! • Over the past 10 years, ASTM and NIST are discussing standards requiring 66% of yield strength maintained after 20 minutes at 600°C. Photo credit: Purdue Engineers Test Effects of Fire on Steel Structures. Homel. Secur. News Wire (2010). at <http://www.homelandsecuritynewswire.com/purdue-engineers-test-effects-fire-steel-structures> 3 Fire resistant versus “normal” steel • ! Delay onset of thermally activated failure processes.! • Enhanced safety for building occupants.! • Reduces need for volatile and labor intensive Fig. 5. insulation. Fire resistant steel Fire,resistant! steel! Normal steel Normal!structural! steel! Temperature! Temperature dependence of yield strength of normal structural and fire-resistant steels Courtesy of Prof. Yip-Wah Chung 4 Incoherent versus coherent precipitates • • • • (Nb,V) carbonitrides form with a Baker-Nutting relationship. Pure NbC carbides have less than a 10% mismatch between lattice planes. (Nb,V) carbonitrides have less than a 6% mismatch. Misfit dislocations arise in semicoherent interfaces. Image credit: Grote, K-H and Erik Antonsson. Springer Handbook of Mechanical Engineering. Springer-Verlag 2009. 5 Design objectives • Primary: • Meet or exceed proposed standards by designing a steel that maintains over 66% of the room temperature yield strength after 20 minutes of exposure at 600°C.! ! • • Room temperature yield strength of at least 350 MPa.! Secondary: • • • Alloy content of V + Nb + Mo < 0.55 wt. %.! Carbon content < 0.1 wt. %.! No water or oil quench or thermo-mechanical processing. 6 Design strategies • Form small, Nb and V based monocarbide (MC) precipitates.! • Reduce or eliminate higher order carbides and cementite to allow maximum MC formation.! • Use thermodynamic modeling to guide design process. 7 Systems design chart 8 Thermodynamic modeling All compositions in wt. % Base Alloy Increased Cr Increased C Base Alloy: 0.05-C 0.25-Cr 0.15-Mo 0.07-Nb 9 Experimental alloys • Two commercial alloys, FR-5 and FR-6, supplied by Nucor.! • FR-7 created by arc melting FR-5 with C and V additions. Supplied by Sophisticated Alloys. FR-7 100 µm 10 Experimental alloy compositions FR-6 11 Local electron atom probe (LEAP) experiments • LEAP was used to investigate the presence of carbide precipitates.! • Size, distribution, and composition can be determined from the LEAP reconstruction. Photo Credit: NUCAPT 12 FR-5: Atom probe result from air-cooled sample Only Nb & C atoms are shown 13 FR-5: Atom probe result from aging for 2 hours at 600°C Only Nb & C atoms are shown Evidence of clusters 1 nm in radius or less! (about 100 atoms) 14 FR-5: Carbon clustering between 0 and 2 hours Air cooled After 2 hrs at 600°C C negligible clustering C observable clustering 15 FR-5: Atom probe result from aging for 6 hours at 600°C Nb, C precipitates Only 50% of Nb & C atoms are shown! ! 1% Nb isosurfacing and 1% C isosurfacing shown to emphasize precipitates 16 Existence of two types of precipitates based on (C+N)/M ratio M = Cr + Mo + V + Nb M2C MC MC M2C 17 Composition profiles of typical precipitates MC M2C Nb 40 20 Concentration of N, C, V, Cr, and Nb in at. % 20 Concentration of N, C, V, Cr, and Nb in at. % Nb 40 0 Cr 40 20 0 V 40 20 0 C 40 20 0 N 40 0 20 0 20 0 20 0 0 3 4 Distance (nm) 5 6 N 40 0 2 C 40 20 1 V 40 20 0 Cr 40 0 1 2 3 4 Distance (nm) 5 6 18 Composition comparison with Thermo-Calc MC precipitate composition 19 Mechanical Testing Parameters • Conducted • Strain in accordance with ASTM standards.! rate 0.005 ± 0.002 1/min.! • High temperature tensile tests conducted in atmosphere.! • High temperature compression tests conducted under controlled environment. 20 Experimental alloy compositions FR-6 21 FR-5: Stress-strain curves at 20°C and 600°C (held for 20 min) Tension FR-5 Yield strength (YS) ratio 0.67 ± 0.06 Compression FR-5 YS ratio 0.64 ± 0.03 22 FR-6: Tensile curves at 20°C and 600°C (held for 20 min) YS ratio 0.50 ± 0.02 23 FR-7: Compression curves at 20°C and 600°C (held for 20 min) FR-7 YS ratio 0.72 ± 0.03 24 Alloy Compositions FR-7 FR-8 supplied by Sophisticated Alloys 25 FR-8 Isopleth FR-8 26 MC phase fraction contributes to high temperature strength Calculated equilibrium carbide phase fraction 27 FR-8: Compression curves at 20°C and 600°C YS ratio 0.71 ± 0.04 YS ratio 0.81 ± 0.06 28 Initial conclusions and future work • Design process resulted in a steel that exceeded the goal: reaching over 70% YS retention after 20 minutes, and over 80% YS retention after 2 hours of exposure to 600°C.! • Thermo-Calc accurately predicted the composition of small carbonitride precipitates.! • Future work: predict interfacial energy and coherency to optimize precipitate composition. 29 Creep resistant steels for steam turbines • Current Ni based superalloys are expensive.! • Steels currently creep too rapidly to be used for ultra supercritical (USC) steam generators.! • Increasing the operating temperature in USC steam generators will reduce greenhouse gas emissions worldwide. Photo credit: NRC 30 Creep resistant steel alloys for steam turbine applications • Requires at least 9 wt. % Cr for corrosion resistance.! • Creep resistance at 35 MPa at temperatures over 620°C.! • Minimize alloy content to remain cost competitive with current options. Photo credit: General Electric Company. http://www.ge-energy.com/products_and_services/services/steam_turbines_power_generation_services/ 31 Concluding remarks • We have built a foundation of theoretical models that predict experimental observations.! • I have confidence that we will be able to use this design process to achieve the proposed goals.! • The development of an effective steel for steam turbine use has the potential to change the world. 32 Acknowledgments • Professors Morris E. Fine, Yip-Wah Chung, Semyon Vaynman, and Dieter Isheim.! • Dr. Shrikant Bhat for his help and insight! • Nucor and Sophisticated Alloys for providing the alloys.! • The NSF CMMI for supporting the research.! • The OMM, CLAMMP, and NUCAPT facilities at Northwestern University. 33 Thank you! Questions?